Intercellular Instructed-Assembly Mimics Protein Dynamics to Induce Cell Spheroids
Cell-mediated remodeling of extracellular matrix (ECM) plays important roles for cell functions, but it is challenging to develop synthetic materials for mimicking such a dynamic aspect of proteins in ECM. Here we show that intercellular morphological transition of peptide assemblies mimic the unfolding of fibronectin, thus enabling cell to form spheroids from a monolayer of cells. Specifically, the phosphopeptide self-assembles to form nanoparticles, which turns into nanofibers upon partial dephosphorylation catalyzed by enzymes (e.g., phosphatases) at intercellular space. Occurring between HS-5 cells, such an enzyme instructed self-assembly enables a sheet of the HS-5 cells to form cell spheroids. Structure-activity investigation reveals that proteolytic stability, dephosphorylation, and biotin conjugation of the peptides are indispensable for forming the cell spheroids. Further mechanism study indicates that the intercellular assemblies interact with multiple ECM components (e.g., laminin, collagens III and IV) to drive the formation of the cell spheroids. As the first example of intercellular instructed-assembly from homotypic precursors, this work illustrates a new approach that uses cell-responsive peptide assemblies to mimic protein dynamics for control cell behaviors.
<p>Extracellular matrix (ECM) plays multifarious roles in cellular processes, such as proliferation,1 differentiation,2 migration,3 and communication.4 In the development of biomaterials for regenerative medicine and tissue engineering, considerable efforts have centered on designing biomaterials to mimic ECM for guiding the behavior of cells, such as using simple biochemical cues (e.g., cell adhesion sequences) for controlling cell adhesion,5 modulating elasticity of matrix for directing cell differentiation,2,6–7 polyvalent carbohydrates for inhibiting agglutination8 or promoting cell aggregation,9 and applying photochemistry to switch synthetic networks for guiding cell migration and proliferation.10 Despite that significant progresses have achieved by these approaches, most synthetic ECM materials lack the dynamic features exhibited by the proteins that constitute ECM. For example, ECM undergoes cell-mediated remodeling, which play essential physiological roles in regulating tissue architecture, morphogenesis, and homoeostasis.11 Thus, it would be advantageous and necessary to develop a facile approach to generate materials that, like endogenous ECM, undergo cell-mediated remodeling.</p><p>A well-studied example of ECM remodeling is the unfolding of fibronectin (FN), a major ECM glycoprotein that plays central role for regulating a variety of cell activities.12 Initiated by integrin receptor on cell surface, the unfolding of FN assembly is a cell-mediated process: the dimeric globular FN bind with integrin, integrin receptors at focal adhesion sites transmit cellular contraction forces, and this local mechanical change of the cell stretches FN molecules to active conformations, and thus promoting FN-FN interactions to form fibrils. The increase of noncovalent interactions between the fibrils further stabilizes the fibrillar networks to enhance fibrillar adhesions.13 Occurring at the intercellular space, such a fibrillar adhesion provides cell-cell adhesive forces that are critical for 2D to 3D cell morphogenesis in vitro.14 So the essence of FN unfolding is to generate cell adhesion force by forming FN fibrils from globular FN. Since the determinant for cell morphogenesis is biophysical in nature (i.e., cell-cell adhesive forces),14 it should be feasible to use molecules other than FN to modulate cell adhesion forces for generating cell spheroids. Stimulated by this insight,14 we intended to build synthetic fibrillar matrix for modulating cell adhesion forces and inducing cell spheroids.</p><p>To mimic the essence of FN unfolding and to ensure the mediation by the cells, we decided to use instructed-assembly15–18 to form supramolecular nanofibers at intercellular space as the synthetic fibrillar matrix (Scheme 1). To maintain the adhesion of the nanofibers with the cells and to distinct from the endogenous cell adhesion motifs (e.g., RGD, IKVAV, YIGSR, and carbohydrates),19–22 we used biotin as the proteolytic resistant cell adhesion motif because various cell lines express high level biotin receptor.23 So we designed a biotinylated D-phosphotetrapeptide (pD1-B) as the substrate for the phosphatase instructed assembly. Our studies show that, being partially dephosphorylated by phosphatases at intercellular space, globular assemblies (i.e., nanoparticles) of pD1-B turns into nanofibers (consisting of the mixture of pD1-B and D1-B) at the intercellular space, which transforms a 2D cell sheet to 3D cell spheroids. Dephosphorylation, cell surface binding motif, and proteolytic resistance of the precursor, are essential for the observed cell spheroids. The formed intercellular assemblies interact with multiple ECM components (e.g., laminin, collagens III and IV) within the cell spheroids. As a demonstration of morphological transition of supramolecular assemblies to modulate intercellular mechanical force, this work illustrates a versatile approach that uses enzymatic noncovalent synthesis to mimic protein dynamics and to control biophysical determinants locally for cellular signal transductions.</p><p>As shown in Scheme 1, pD1-B consists of three key components: a well-studied self-assembling backbone (i.e., a diphenylalanine capped with naphthalene (Nap-ff)24), an enzymatic trigger (i.e., tyrosine phosphate (py) as a substrate of phosphatase25–26), and a cell surface targeting motif (i.e., biotin). We utilized biotin because biotin is a ligand of cell surface receptor and is a biocompatible vitamin.23,27 After synthesizing Fmoc (9-fluorenylmethoxycarbonyl) protected phosphorylated tyrosine via two steps, we synthesized Nap-ffkpy by standard solid-phase (Fmoc) peptide chemistry, and subsequently using N-hydroxysuccinimide (NHS) activated biotin to react with Nap-ffkpy via ε-amino group of lysine to form stable amide bonds to result in pD1-B. After purifying the precursor, we used 1H-NMR and LC-MS to confirm their purity and identity. This facile synthetic route (Scheme S1) produces pD1-B in a good yield (76%).</p><p>After demonstrating pD1-B is innocuous to HS-5 cells (Figure S1), we investigated the 3D cell spheroid formation of HS-5 cells upon the treatment of pD1-B. We chose HS-5 cells because these fibroblast cells express relatively low level of phosphatases, synthesize 3D ECM slowly (several days at higher density),28 and serve as a stromal cell line for co-culturing with other disease-related cells. After being treated with pD1-B for 24 h, HS-5 cells form 3D cell spheroids (Figure 1B, S2 and S3) from a 2D cell sheet, while the cells remain a 2D sheet without pD1-B in the culture medium. Adding pD1 or D1-B (Scheme S2), which is the analogue of pD1-B without either the biotin motif or the phosphate group, HS-5 cells remain as a 2D cell sheet. These results indicates that both the binding to cell surface and the dynamic change of pD1-B are indispensable for inducing the 3D cell spheroids. Importantly, using biotin molecules to compete with pD1-B to bind the receptors on cell surface blocks the formation of cell spheroids in a concentration dependent manner (Figure 1E and S5), further confirming the crucial role of biotin, as a ligand, for attaching the assemblies of pD1-B on the cell surface to undergo instructed-assembly at the intercellular space. Using pL1-B, the L-enantiomer of pD1-B, results in smaller clusters of cells (Figure 1F and S6), indicating the proteolytic stability (Figure S7 and S8) of the assemblies of pD1-B also play important roles for forming the cell spheroids.</p><p>To verify that the enzymatic dephosphorylation and self-assembly of pD1-B on the cells are a dynamic process, we quantified the conversion of pD1-B after incubating it with HS-5 cells at different time points. The results (Figure 2A) show that endogenous phosphatases convert 19.2%, 39.5%, and 68.5% of pD1-B to D1-B at 3, 8, and 24 h, respectively. The results indicate that the process of instructed-assembly15 involves two build blocks, pD1-B and D1-B, which co-assemble to form a continuum phosphorylated nanostructures at intercellular space. We next used FITC-avidin to stain the assemblies of pD1-B and D1-B. Figure 2B (and Figure S9) indicates that the fluorescence of FITC-avidin distribute on cell surface as puncta with slightly different sizes, suggesting that the assemblies anchor on cell surface and form intercellular assemblies. In contrast, HS-5 cells treated with pL1-B exhibit very weak fluorescence in cytoplasm, indicating the stability of molecule is important for its anchoring on cell surface. To directly visualize the distribution of these intercellular assemblies, we introduced a nitrobenzofurazan (NBD)-capped phosphopeptide (NBD1P-B, scheme S3) since NBD fluoresces intensely when forming assemblies.29 3D construction of CLSM images (Figure 2C and Video clip S1) reveals that most fluorescent puncta locate around cells, confirming that the intercellular dynamic assemblies of NBD1P-B drive the formation of the cell spheroids.</p><p>We used immunofluorescent staining to detect the co-localization of the assemblies of NBD1P-B and NBD1-B and major components of ECM or cell adhesion molecules. The results reveal that the assemblies partially co-localize with laminin, collagen III, and collagen IV (Figure 2D, video clips S2–S4). The assemblies hardly co-localize with fibronectin. These results imply that intercellular instructed-assembly likely acts as a dynamic adhesive force for generating 3D cell spheroids. Further mechanistic studies (Figure 2D) exclude the direct interaction between the assemblies and cell adhesion molecules, such as N-cadherin and integrins. More importantly, antibodies against α5 (fibronectin receptor) show brighter fluorescence in spheroid (Figure 2D) than in the corresponding 2D cell culture (Figure S10), and antibodies against αvβ3 (vitronectin receptor) exhibit weaker fluorescence in 3D spheroid than in 2D cell culture. These results suggest the transformation of focal adhesion to fibrillar adhesion during cell spheroid formation, which is likely to evolve 3D-matrix adhesion.28,30 Collectively, these results support that intercellular instructed-assembly of small molecules effectively enhancing cell-cell interactions to form 3D cell spheroids.</p><p>Transmission electron microscopy (TEM) helps infer the morphological transformation that likely occurs during intercellular instructed-assembly. pD1-B self-assembles to form relatively uniform nanoparticles (Figure 3A) with diameter of 7±2 nm in aqueous solution, which transform to nanofibers (Figure 3B) with several hundred nanometers in length and 7±2 in width upon the treatment of ectophosphatase (e.g., alkaline phosphatase (ALP)). Similar to pD1-B, adding pL1-B in aqueous solution results in nanoparticles with diameter of 5±2 nm, and then turn into filaments with 3±2 nm in width after addition of ALP (Figure S11). As a control, pD1 forms predominately worm like structures with about 36±2 nm in length and 6±2 nm in width (Figure S12), plus some nanospheres with diameter of 5±2 nm. Upon the addition of ALP, these worm like structures transform to short filaments with 58±2 in length and 5±2 in width (Figure S12). Directly dissolving D1-B in aqueous solution results in uniform nanofibers (Figure S13). These results not only indicate the influence of biotin on the morphology of pD1-B, but also confirm the morphology transition due to dephosphorylation. Such a dynamic, morphological change, reminiscing the cell-mediated dynamics of fibronectin (i.e., from globular to fibril structures during unfolding processes), is the key factor for inducing the cell spheroids.</p><p>Gold-avidin staining (Figure 3C and S14) indicates that biotin presents on the surface of nanofibers, being similar to a previous report,31 suggesting that biotin not only acts as a ligand for anchoring pD1-B on cell surface, but also provides additional hydrogen bonding for intercellular fibrillar interaction to reinforce ECM. Moreover, liquid chromatography mass spectrometry (LC-MS) reveals that the assemblies of pD1-B was dephosphorylated in different rates upon addition of different amounts of ALPs (Figure 3D). Specifically, 0.1 U/mL of ALP hydrolysis pD1-B is much faster than 0.01 U/mL of ALP does, with t½ to be 0.14 and 1.72 h for 0.1 U/mL and 0.01 U/mL of ALP, respectively. This result is consistent with the fact that pD1-B induces the spheroid formation of HS-5 cells, while hardly change the morphology of Saos-2 cells that express higher level of ALP (Figure S15).</p><p>In summary, this work describes that intercellular enzymatic formation of higher-order nanostructures of peptides for controlling the collective behavior of cells. Use only one type of precursor to induce cell spheroid formation, the strategy illustrated in this work is simpler and more general than previous works,32–33 which require two types of molecules (i.e., vancomycin and phosphopeptide). Similarly to the cases of heterotypic precursors, the rate of dephosphorylation likely dictates the formation of the peptide assemblies for forming cell spheroids. Introducing ligands (e.g., biotin) of cell surface receptor for instructed-assembly ensures locally controlling phase transition of assemblies on cell surface, which further influences the mechanical signaling locally for remodeling ECM11 to induce cell morphogenesis. Providing a facile strategy for in-situ constructing molecular assemblies to generate organoids, this work illustrates that spatiotemporal control of noncovalent (or supramolecular) interactions, and it ultimately may contribute to tissue engineering and stem cell therapies.34 Using other functional small molecules instead of biotin in instructed-assembly may lead to novel functions of supramolecular assemblies.</p>